LMucko/crystallography-open-database huggingface dataset:
Structural peculiarities of Bi La2 O4.5+d examined by X-ray and neutron powder diffraction
Wolcyrz, M.; Horyn, R.; Bouree, F.; Journal of Physics: Condensed Matter 11 (1999) 5757–5765; doi:

data_1522187
_publ_section_title
;
 Structural peculiarities of Bi La2 O4.5+d examined by X-ray and neutron
 powder diffraction
;
_journal_name_full               'Journal of Physics: Condensed Matter'
_journal_page_first              5757
_journal_page_last               5765
_journal_volume                  11
_journal_year                    1999
_chemical_formula_sum            'Bi0.667 La1.333 O3.364'
_chemical_name_systematic        '(Bi0.667 La1.333) O3.364'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                87.57
_cell_angle_beta                 90.3
_cell_angle_gamma                90.14
_cell_formula_units_Z            1
_cell_length_a                   3.918
_cell_length_b                   4.024
_cell_length_c                   5.629
_cell_volume                     88.666
_citation_journal_id_ASTM        JCOMEL
_cod_data_source_file            Wolcyrz_JCOMEL_1999_100.cif
_cod_data_source_block           Bi0.667La1.333O3.364
_cod_original_cell_volume        88.66576
_cod_database_code               1522187
Strukturuntersuchungen in den Systemen Ti-Pd und Ti-Pt
Krautwasser, P.; Schubert, K.; Bhan, S.; Zeitschrift fuer Metallkunde 59 (1968) 724–729; doi:

data_1522188
_publ_section_title
;
 Strukturuntersuchungen in den Systemen Ti-Pd und Ti-Pt
;
_journal_name_full               'Zeitschrift fuer Metallkunde'
_journal_page_first              724
_journal_page_last               729
_journal_volume                  59
_journal_year                    1968
_chemical_formula_sum            'Pd3 Ti2'
_space_group_IT_number           63
_symmetry_space_group_name_Hall  '-C 2c 2'
_symmetry_space_group_name_H-M   'C m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   14.33
_cell_length_b                   4.64
_cell_length_c                   4.61
_cell_volume                     306.524
_citation_journal_id_ASTM        ZEMTAE
_cod_data_source_file            Krautwasser_ZEMTAE_1968_1786.cif
_cod_data_source_block           Pd3Ti2
_cod_original_cell_volume        306.5244
_cod_database_code               1522188
Structural peculiarities of Bi La2 O4.5+d examined by X-ray and neutron powder diffraction
Wolcyrz, M.; Horyn, R.; Bouree, F.; Journal of Physics: Condensed Matter 11 (1999) 5757–5765; doi:

data_1522189
_publ_section_title
;
 Structural peculiarities of Bi La2 O4.5+d examined by X-ray and neutron
 powder diffraction
;
_journal_name_full               'Journal of Physics: Condensed Matter'
_journal_page_first              5757
_journal_page_last               5765
_journal_volume                  11
_journal_year                    1999
_chemical_formula_sum            'Bi La2 O4.5'
_chemical_name_systematic        '(Bi La2) O4.5'
_space_group_IT_number           160
_symmetry_space_group_name_Hall  'R 3 -2"'
_symmetry_space_group_name_H-M   'R 3 m :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            1
_cell_length_a                   3.966
_cell_length_b                   3.966
_cell_length_c                   9.931
_cell_volume                     135.279
_citation_journal_id_ASTM        JCOMEL
_cod_data_source_file            Wolcyrz_JCOMEL_1999_98.cif
_cod_data_source_block           Bi1La2O4.5
_cod_original_cell_volume        135.2786
_cod_original_formula_sum        'Bi1 La2 O4.5'
_cod_database_code               1522189
Strukturuntersuchungen in den Systemen Ti-Pd und Ti-Pt
Krautwasser, P.; Schubert, K.; Bhan, S.; Zeitschrift fuer Metallkunde 59 (1968) 724–729; doi:

data_1522190
_publ_section_title
;
 Strukturuntersuchungen in den Systemen Ti-Pd und Ti-Pt
;
_journal_name_full               'Zeitschrift fuer Metallkunde'
_journal_page_first              724
_journal_page_last               729
_journal_volume                  59
_journal_year                    1968
_chemical_formula_sum            'Pd5 Ti3'
_space_group_IT_number           123
_symmetry_space_group_name_Hall  '-P 4 2'
_symmetry_space_group_name_H-M   'P 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.263
_cell_length_b                   3.263
_cell_length_c                   11.436
_cell_volume                     121.761
_citation_journal_id_ASTM        ZEMTAE
_cod_data_source_file            Krautwasser_ZEMTAE_1968_1787.cif
_cod_data_source_block           Pd5Ti3
_cod_database_code               1522190
Structural peculiarities of Bi La2 O4.5+d examined by X-ray and neutron powder diffraction
Wolcyrz, M.; Horyn, R.; Bouree, F.; Journal of Physics: Condensed Matter 11 (1999) 5757–5765; doi:

data_1522191
_publ_section_title
;
 Structural peculiarities of Bi La2 O4.5+d examined by X-ray and neutron
 powder diffraction
;
_journal_name_full               'Journal of Physics: Condensed Matter'
_journal_page_first              5757
_journal_page_last               5765
_journal_volume                  11
_journal_year                    1999
_chemical_formula_sum            'Bi0.667 La1.333 O3'
_chemical_name_systematic        '(Bi0.667 La1.333) O3'
_space_group_IT_number           12
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_cell_angle_alpha                90
_cell_angle_beta                 125.11
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   6.826
_cell_length_b                   3.987
_cell_length_c                   4.051
_cell_volume                     90.189
_citation_journal_id_ASTM        JCOMEL
_cod_data_source_file            Wolcyrz_JCOMEL_1999_99.cif
_cod_data_source_block           Bi0.667La1.333O3
_cod_original_cell_volume        90.18915
_cod_database_code               1522191
Strukturuntersuchungen in den Systemen Ti-Pd und Ti-Pt
Krautwasser, P.; Bhan, S.; Schubert, K.; Zeitschrift fuer Metallkunde 59 (1968) 724–729; doi:

data_1522192
_publ_section_title
;
 Strukturuntersuchungen in den Systemen Ti-Pd und Ti-Pt
;
_journal_name_full               'Zeitschrift fuer Metallkunde'
_journal_page_first              724
_journal_page_last               729
_journal_volume                  59
_journal_year                    1968
_chemical_formula_sum            'Pt5 Ti3'
_space_group_IT_number           72
_symmetry_space_group_name_Hall  '-I 2 2c'
_symmetry_space_group_name_H-M   'I b a m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.953
_cell_length_b                   5.441
_cell_length_c                   8.169
_cell_volume                     486.834
_citation_journal_id_ASTM        ZEMTAE
_cod_data_source_file            Krautwasser_ZEMTAE_1968_1860.cif
_cod_data_source_block           Pt5Ti3
_cod_original_cell_volume        486.8338
_cod_database_code               1522192
Investigation of (Sr4-d Cad) Pt O6 using X-ray Rietveld refinement
Wong-Ng, W.; Young, R.A.; Kaduk, J.A.; Jiang, F.; Swartzendruber, L.J.; Brown, H.J.; Powder Diffraction 14 (1999) 181–189; doi:

data_1522193
_publ_section_title
;
 Investigation of (Sr4-d Cad) Pt O6 using X-ray Rietveld refinement
;
_journal_name_full               'Powder Diffraction'
_journal_page_first              181
_journal_page_last               189
_journal_volume                  14
_journal_year                    1999
_chemical_formula_sum            'O6 Pt Sr4'
_chemical_name_systematic        'Sr4 Pt O6'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   9.7477
_cell_length_b                   9.7477
_cell_length_c                   11.8791
_cell_volume                     977.504
_citation_journal_id_ASTM        PODIE2
_cod_data_source_file            Wong-Ng_PODIE2_1999_680.cif
_cod_data_source_block           O6Pt1Sr4
_cod_original_cell_volume        977.5038
_cod_original_formula_sum        'O6 Pt1 Sr4'
_cod_database_code               1522193
Darstellung und Struktur von Na4 Ge2 S6 (H2 O)14 und Na4 Sn2 S6 (H2 O)14
Krebs, B.; Pohl, S.; Schiwy, W.; Zeitschrift fuer Anorganische und Allgemeine Chemie 393 (1972) 241–252; doi:

data_1522194
_publ_section_title
;
 Darstellung und Struktur von Na4 Ge2 S6 (H2 O)14 und Na4 Sn2 S6 (H2 O)14
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              241
_journal_page_last               252
_journal_volume                  393
_journal_year                    1972
_chemical_formula_sum            'Ge2 H28 Na4 O14 S6'
_chemical_name_systematic        'Na4 Ge2 S6 (H2 O)14'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                108.41
_cell_angle_beta                 92.39
_cell_angle_gamma                91.69
_cell_formula_units_Z            1
_cell_length_a                   9.978
_cell_length_b                   7.02
_cell_length_c                   9.601
_cell_volume                     636.888
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Krebs_ZAACAB_1972_35.cif
_cod_data_source_block           H28Ge2Na4O14S6
_cod_original_cell_volume        636.8881
_cod_original_formula_sum        'H28 Ge2 Na4 O14 S6'
_cod_database_code               1522194
Investigation of (Sr4-d Cad) Pt O6 using X-ray Rietveld refinement
Wong-Ng, W.; Swartzendruber, L.J.; Kaduk, J.A.; Brown, H.J.; Young, R.A.; Jiang, F.; Powder Diffraction 14 (1999) 181–189; doi:

data_1522195
_publ_section_title
;
 Investigation of (Sr4-d Cad) Pt O6 using X-ray Rietveld refinement
;
_journal_name_full               'Powder Diffraction'
_journal_page_first              181
_journal_page_last               189
_journal_volume                  14
_journal_year                    1999
_chemical_formula_sum            'Ca0.85 O6 Pt Sr3.15'
_chemical_name_systematic        '(Sr3.15 Ca0.85) Pt O6'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   9.724
_cell_length_b                   9.724
_cell_length_c                   11.5214
_cell_volume                     943.465
_citation_journal_id_ASTM        PODIE2
_cod_data_source_file            Wong-Ng_PODIE2_1999_681.cif
_cod_data_source_block           Ca0.85O6Pt1Sr3.15
_cod_original_formula_sum        'Ca0.85 O6 Pt1 Sr3.15'
_cod_database_code               1522195
Darstellung und Struktur von Na4 Sn2 S6 (H2 O)14 und Na4 Sn2 S6 (H2 O)14
Krebs, B.; Schiwy, W.; Pohl, S.; Zeitschrift fuer Anorganische und Allgemeine Chemie 393 (1972) 241–252; doi:

data_1522196
_publ_section_title
;
 Darstellung und Struktur von Na4 Sn2 S6 (H2 O)14 und Na4 Sn2 S6 (H2 O)14
;
_journal_name_full
'Zeitschrift fuer Anorganische und Allgemeine Chemie'
_journal_page_first              241
_journal_page_last               252
_journal_volume                  393
_journal_year                    1972
_chemical_formula_sum            'H28 Na4 O14 S6 Sn2'
_chemical_name_systematic        'Na4 Sn2 S6 (H2 O)14'
_space_group_IT_number           2
_symmetry_space_group_name_Hall  '-P 1'
_symmetry_space_group_name_H-M   'P -1'
_cell_angle_alpha                108.3
_cell_angle_beta                 92.18
_cell_angle_gamma                91.11
_cell_formula_units_Z            1
_cell_length_a                   10.114
_cell_length_b                   7.027
_cell_length_c                   9.801
_cell_volume                     660.500
_citation_journal_id_ASTM        ZAACAB
_cod_data_source_file            Krebs_ZAACAB_1972_43.cif
_cod_data_source_block           H28Na4O14S6Sn2
_cod_original_cell_volume        660.5003
_cod_database_code               1522196
Investigation of (Sr4-d Cad) Pt O6 using X-ray Rietveld refinement
Wong-Ng, W.; Kaduk, J.A.; Young, R.A.; Jiang, F.; Swartzendruber, L.J.; Brown, H.J.; Powder Diffraction 14 (1999) 181–189; doi:

data_1522197
_publ_section_title
;
 Investigation of (Sr4-d Cad) Pt O6 using X-ray Rietveld refinement
;
_journal_name_full               'Powder Diffraction'
_journal_page_first              181
_journal_page_last               189
_journal_volume                  14
_journal_year                    1999
_chemical_formula_sum            'Ca1.855 O6 Pt Sr2.145'
_chemical_name_systematic        '(Sr2.145 Ca1.855) Pt O6'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   9.6153
_cell_length_b                   9.6153
_cell_length_c                   11.4284
_cell_volume                     915.044
_citation_journal_id_ASTM        PODIE2
_cod_data_source_file            Wong-Ng_PODIE2_1999_682.cif
_cod_data_source_block           Ca1.855O6Pt1Sr2.145
_cod_original_cell_volume        915.0435
_cod_original_formula_sum        'Ca1.855 O6 Pt1 Sr2.145'
_cod_database_code               1522197
Phase equilibria in the Nb-V-Ga system at 800 deg. C
Kreidenko, F.S.; Markiv, V.Ya.; Sokolovskaya, E.M.; Vestnik Moskovskogo Universiteta, Khimiya 15 (1974) 748–750; doi:

data_1522198
_publ_section_title
;
 Phase equilibria in the Nb-V-Ga system at 800 deg. C
;
_journal_name_full               'Vestnik Moskovskogo Universiteta, Khimiya'
_journal_page_first              748
_journal_page_last               750
_journal_volume                  15
_journal_year                    1974
_chemical_formula_sum            'Ga Nb1.8 V1.2'
_chemical_name_systematic        'Ga (Nb0.6 V0.4)3'
_space_group_IT_number           223
_symmetry_space_group_name_Hall  '-P 4n 2 3'
_symmetry_space_group_name_H-M   'P m -3 n'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   5.05
_cell_length_b                   5.05
_cell_length_c                   5.05
_cell_volume                     128.788
_citation_journal_id_ASTM        VMUKA5
_cod_data_source_file            Kreidenko_VMUKA5_1974_247.cif
_cod_data_source_block           Ga1Nb1.8V1.2
_cod_original_cell_volume        128.7876
_cod_original_formula_sum        'Ga1 Nb1.8 V1.2'
_cod_database_code               1522198
Investigation of (Sr4-d Cad) Pt O6 using X-ray Rietveld refinement
Wong-Ng, W.; Brown, H.J.; Kaduk, J.A.; Jiang, F.; Young, R.A.; Swartzendruber, L.J.; Powder Diffraction 14 (1999) 181–189; doi:

data_1522199
_publ_section_title
;
 Investigation of (Sr4-d Cad) Pt O6 using X-ray Rietveld refinement
;
_journal_name_full               'Powder Diffraction'
_journal_page_first              181
_journal_page_last               189
_journal_volume                  14
_journal_year                    1999
_chemical_formula_sum            'Ca2.906 O6 Pt Sr1.094'
_chemical_name_systematic        '(Sr1.094 Ca2.906) Pt O6'
_space_group_IT_number           167
_symmetry_space_group_name_Hall  '-R 3 2"c'
_symmetry_space_group_name_H-M   'R -3 c :H'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            6
_cell_length_a                   9.478
_cell_length_b                   9.478
_cell_length_c                   11.3301
_cell_volume                     881.450
_citation_journal_id_ASTM        PODIE2
_cod_data_source_file            Wong-Ng_PODIE2_1999_683.cif
_cod_data_source_block           Ca2.906O6Pt1Sr1.094
_cod_original_cell_volume        881.4501
_cod_original_formula_sum        'Ca2.906 O6 Pt1 Sr1.094'
_cod_database_code               1522199
Investigation of the first-order magnetic transformation in Mn3 Pt
Kren, E.; Kadar, G.; Pal, L.; Szabo, P.; Journal of Applied Physics 38 (1967) 1265–1266; doi:

data_1522200
_publ_section_title
;
 Investigation of the first-order magnetic transformation in Mn3 Pt
;
_journal_name_full               'Journal of Applied Physics'
_journal_page_first              1265
_journal_page_last               1266
_journal_volume                  38
_journal_year                    1967
_chemical_formula_sum            'Mn3 Pt0.5 Rh0.5'
_chemical_name_systematic        'Mn3 (Pt0.5 Rh0.5)'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.82
_cell_length_b                   3.82
_cell_length_c                   3.82
_cell_volume                     55.743
_citation_journal_id_ASTM        JAPIAU
_cod_data_source_file            Kren_JAPIAU_1967_1157.cif
_cod_data_source_block           Mn3Pt0.5Rh0.5
_cod_original_cell_volume        55.74297
_cod_database_code               1522200
Negative thermal expansion in Y2 (W O4)3
Woodcock, D.A.; Ritter, C.; Lightfoot, P.; Journal of Solid State Chemistry 149 (2000) 92–98; doi:

data_1522201
_publ_section_title
;
 Negative thermal expansion in Y2 (W O4)3
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              92
_journal_page_last               98
_journal_volume                  149
_journal_year                    2000
_chemical_formula_sum            'Al2 O12 W3'
_chemical_name_systematic        'Al2 (W O4)3'
_space_group_IT_number           60
_symmetry_space_group_name_Hall  '-P 2a 2n'
_symmetry_space_group_name_H-M   'P n c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   9.1364
_cell_length_b                   12.5913
_cell_length_c                   9.056
_cell_volume                     1041.795
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Woodcock_JSSCBI_2000_1747.cif
_cod_data_source_block           Al2O12W3
_cod_original_sg_symbol_Hall     '-P 2n 2ab (z,x,y)'
_cod_database_code               1522201
Magnetic structures and exchange interactions in the Mn-Pt system
Kren, E.; Kadar, G.; Tarnoczi, T.; Pal, L.; Solyom, J.; Szabo, P.; Physical Review (1,1893-132,1963/141,1966-188,1969) 171 (1968) 574–585; doi:

data_1522202
_publ_section_title
;
 Magnetic structures and exchange interactions in the Mn-Pt system
;
_journal_name_full
'Physical Review (1,1893-132,1963/141,1966-188,1969)'
_journal_page_first              574
_journal_page_last               585
_journal_volume                  171
_journal_year                    1968
_chemical_formula_sum            'Mn3 Pt'
_space_group_IT_number           221
_symmetry_space_group_name_Hall  '-P 4 2 3'
_symmetry_space_group_name_H-M   'P m -3 m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            1
_cell_length_a                   3.833
_cell_length_b                   3.833
_cell_length_c                   3.833
_cell_volume                     56.314
_citation_journal_id_ASTM        PHRVAO
_cod_data_source_file            Kren_PHRVAO_1968_1156.cif
_cod_data_source_block           Mn3Pt1
_cod_original_cell_volume        56.31401
_cod_original_formula_sum        'Mn3 Pt1'
_cod_database_code               1522202
Neutron diffraction study of Mn3 Ga
Kren, E.; Kadar, G.; Solid State Communications 8 (1970) 1653–1655; doi:

data_1522203
_publ_section_title
;
 Neutron diffraction study of Mn3 Ga
;
_journal_name_full               'Solid State Communications'
_journal_page_first              1653
_journal_page_last               1655
_journal_volume                  8
_journal_year                    1970
_chemical_formula_sum            'Ga1.15 Mn2.85'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   3.901
_cell_length_b                   3.901
_cell_length_c                   7.12
_cell_volume                     108.351
_citation_journal_id_ASTM        SSCOA4
_cod_data_source_file            Kren_SSCOA4_1970_212.cif
_cod_data_source_block           Ga1.15Mn2.85
_cod_original_cell_volume        108.3507
_cod_database_code               1522203
Negative thermal expansion in Y2 (W O4)3
Woodcock, D.A.; Lightfoot, P.; Ritter, C.; Journal of Solid State Chemistry 149 (2000) 92–98; doi:

data_1522204
_publ_section_title
;
 Negative thermal expansion in Y2 (W O4)3
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              92
_journal_page_last               98
_journal_volume                  149
_journal_year                    2000
_chemical_formula_sum            'O12 W3 Y2'
_chemical_name_systematic        'Y2 (W O4)3'
_space_group_IT_number           60
_symmetry_space_group_name_Hall  '-P 2a 2n'
_symmetry_space_group_name_H-M   'P n c a'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   10.07
_cell_length_b                   13.937
_cell_length_c                   9.98
_cell_volume                     1400.649
_citation_journal_id_ASTM        JSSCBI
_cod_data_source_file            Woodcock_JSSCBI_2000_1749.cif
_cod_data_source_block           O12W3Y2
_cod_original_sg_symbol_Hall     '-P 2n 2ab (z,x,y)'
_cod_database_code               1522204
Neutron diffraction experiments on U Cu4+x Al8-x
Krimmel, A.; Loidl, A.; McIntyre, G.J.; Geibel, C.; Steglich, F.; Journal of Magnetism and Magnetic Materials 103 (1992) 73–77; doi:

data_1522205
_publ_section_title
;
 Neutron diffraction experiments on U Cu4+x Al8-x
;
_journal_name_full               'Journal of Magnetism and Magnetic Materials'
_journal_page_first              73
_journal_page_last               77
_journal_volume                  103
_journal_year                    1992
_chemical_formula_sum            'Al7 Cu5 U'
_chemical_name_systematic        '(Al7 Cu5) U'
_space_group_IT_number           139
_symmetry_space_group_name_Hall  '-I 4 2'
_symmetry_space_group_name_H-M   'I 4/m m m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.698
_cell_length_b                   8.698
_cell_length_c                   5.081
_cell_volume                     384.404
_citation_journal_id_ASTM        JMMMDC
_cod_data_source_file            Krimmel_JMMMDC_1992_1208.cif
_cod_data_source_block           Al7Cu5U1
_cod_original_cell_volume        384.4041
_cod_original_formula_sum        'Al7 Cu5 U1'
_cod_database_code               1522205